Advances in Condensed Matter Physics

Volume 2013 (2013), Article ID 286325, 5 pages

http://dx.doi.org/10.1155/2013/286325

## Thermodynamic, Electromagnetic, and Lattice Properties of Antiperovskite Mn_{3}SbN

^{1}International Center for Materials Nanoarchitectonics (WPI-MANA), National Institute for Materials Science, 1-1 Namiki, Ibaraki, Tsukuba 305-0044, Japan^{2}Superconducting Properties Unit, National Institute for Materials Science, 1-1 Namiki, Ibaraki, Tsukuba 305-0044, Japan^{3}Materials Processing Unit, National Institute for Materials Science, 1-1 Namiki, Ibaraki, Tsukuba 305-0044, Japan^{4}Graduate School of Chemical Sciences and Engineering, Hokkaido University, Hokkaido, Sapporo 060-0810, Japan^{5}Department of Physics, Center for Condensed Matter and Materials Physics, Beihang University, Beijing, Haidian 100191, China

Received 1 October 2012; Revised 4 December 2012; Accepted 5 December 2012

Academic Editor: Y. Sun

Copyright © 2013 Ying Sun et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

#### Abstract

The physical properties of polycrystalline Mn_{3}SbN were investigated using measurements of the magnetic, calorimetric, and electronic transport properties. At room temperature, the phase crystallizes in a tetragonal structure with symmetry. A remarkably sharp peak in the heat capacity versus temperature curve was found near 353 K. The peak reaches 723 J mol^{−1} K^{−1} at its highest, which corresponds to a transition entropy of 10.2 J mol^{−1} K^{−1}. The majority of the large entropy change appears to be due to lattice distortion from the high-temperature cubic structure to the room-temperature tetragonal structure and the accompanying Ferrimagnetic transition.

#### 1. Introduction

Antiperovskite compounds with the formula Mn_{3}XN or Mn_{3}XC (X = Cu, Zn, Ga, Cu, In, or Sn) were discovered in the middle of the last century [1]. Recently, interest in these materials has intensively renewed owing to discoveries of new, potentially useful properties [2–4] such as the giant magnetoresistance of Mn_{3}GaC [5], negative thermal expansion (NTE) of Mn_{3}Cu(Ge)N [6] and Mn_{3}Zn(Ge)N [7], magnetostriction of Mn_{3}CuN [8] and Mn_{3}SbN [9], and near-zero temperature coefficient of the resistivity of Mn_{3}CuN [10] and Mn_{3}NiN [11]. Specifically, Takenaka and Takagi found that Ge-doped Mn_{3}CuN compound has a large NTE (NTE parameter = −25 × 10^{−6} K^{−1}) [12]; using neutron diffraction, the broad NTE was determined to be associated with the local T_{4} structure [6]. Asano et al. discovered large magnetostriction in tetragonal Mn_{3}CuN; it expands 0.2% and shrinks 0.1% in the directions parallel and perpendicular to an external 90 kOe magnetic field, respectively [8]. In previous studies, we found a peculiar phase separation and accompanying anomaly in the electronic transport properties of Mn_{3}ZnN [13, 14], while further study indicated that the thermal expansion properties of Mn_{3}ZnN can be controlled by introducing Zn vacancies [15]. In addition, Song et al. observed a canonical spin-glass state in Mn_{3}GaN below the spin-freezing temperature of 133 K [16]. Lukashev et al. systematically studied the spin density of the spin-frustrated state of a Mn-based antiperovskite under mechanical stress [17].

The above-mentioned properties enable a variety of potential applications for this type of material. Although the prospective industrial markets are expected to be large and much effort has already been devoted to studying their structural, electromagnetic, and transport properties, further investigations on antiperovskite materials are still required. In this study, the thermodynamic, electromagnetic, and electronic transport properties of Mn_{3}SbN are investigated. In particular, we focused on the notable transition entropy that accompanies the magnetic and crystal structure transition above room temperature.

#### 2. Experimental Details

A polycrystalline Mn_{3}SbN sample was prepared via the solid-state reaction of fine powders of Sb (99.99%, Rare Metallic Co.) and Mn_{2}N, which was synthesized by firing Mn powder (99.99%, Sigma Aldrich Co.) in nitrogen at 800°C for 60 h. Stoichiometric amounts of the starting materials were thoroughly mixed, and the mixture was pressed into a pellet. The pellet was sealed in an evacuated quartz tube, heated in a box furnace at 800°C for three days, and then slowly cooled to room temperature in the furnace.

The crystal structure of Mn_{3}SbN was analyzed by synchrotron X-ray diffraction (SXRD) using a large Debye-Scherrer camera at the BL15XU NIMS beam line of the SPring-8 facility in Hyogo, Japan. The SXRD data were collected for 2*θ* ranging from 2° to 60° at intervals of 0.003°. The incident beam was monochromatized at Å. The evolution of the Mn_{3}SbN crystal structure with temperature was also determined via the measurement of the SXRD patterns.

The temperature dependence of magnetization was measured between 2 and 400 K with applied magnetic fields of 0.1 and 5 kOe using a Magnetic Property Measurements System (Quantum Design). The measurements were conducted on loosely gathered powder under both zero-field cooling (ZFC) and field cooling (FC) conditions. The isothermal magnetization curve was recorded at 10 K between −50 and 50 kOe.

Specific heat () values were measured between 2 and 400 K with cooling using a Physical Properties Measurement System (Quantum Design). The sample was fixed on a stage using a small amount of grease; the heat capacity of the grease was measured first and subtracted from the total .

The electrical resistivity () was measured between 2 and 400 K with cooling and heating using a conventional four-probe techniques with the same apparatus. The AC gauge current and frequency were 10 mA and 30 Hz, respectively. The electrical contacts were prepared on the surface of a bar-shaped piece of the pellet using silver paste and Pt wires.

#### 3. Results and Discussion

As shown in Figure 1, the synchrotron XRD pattern at room temperature fit well with a model pattern of the proposed structure (space group: *P*4*/mmm*). The structural parameters of Mn_{3}SbN were refined by the Rietveld method using the RIETAN-FP program [18]. The occupancy factors of Sb, N, Mn1, and Mn2 were refined to be 1 (fixed), 1 (fixed), 0.97, and 0.99, respectively, while the isotropic atomic displacement parameters were 0.42, 0.84(5), 0.86, and 0.78 Å^{2}, respectively. The lattice constants were calculated to be *a* = *b* = 4.17994(4) Å and *c* = 4.27718(5) Å. The final and reliability indexes were below 5.56% and 4.09%, respectively. The analysis revealed 1.91 mass% MnO in the sample as an impurity; as shown later, the magnetic, , and measurements suggest that the impurity does not significantly impact the measurements of Mn_{3}SbN in this study.

Figure 2 displays the temperature dependence of magnetization of polycrystalline Mn_{3}SbN. The magnetization steeply increases upon cooling to around 353 K, which suggests the establishment of long-range magnetic order at the magnetic transition temperature (). In addition, a small hysteresis can be observed between the heating and cooling process, implying the first-order character of the magnetic transition. The remarkable bifurcation between the ZFC and FC curves may originate from the spontaneous alignment of random magnetic Mn moments in domain boundaries. It is worth noting that the hysteresis is less significant at a higher magnetic field of 5 kOe, which supports the domain picture.

To further study the magnetic properties, we applied the Curie-Weiss law to the paramagnetic portion. As shown in the right inset of Figure 2, the plot is well represented by the Curie-Weiss law, that is, the spin-only expression for magnetic susceptibility: , where is the Curie constant and is the Weiss temperature. The value of was determined to be 354 K, which suggests that ferromagnetic correlation is dominant in the spin system. The effective Bohr magneton () was estimated to be 1.28 /Mn from (C/*η*)^{0.5}, where is the number of magnetic atoms in the molecular formula ( in the present case). The value of is much lower than that of other antiperovskite manganese nitrides (e.g., 2.87 for Mn_{3}ZnN [14]) and even lower than the expected moment for localized spins, suggesting an itinerant character of the 3d electrons in Mn_{3}SbN.

From the isothermal magnetization curve (see the inset of Figure 2), it was found that the magnetization at 50 kOe is ~0.35 /Mn, which is too small to be caused by full ferromagnetic order. The gap suggests that the spins of the Mn atoms are possibly Ferrimagnetically ordered. This Ferrimagnetic interaction is also suggested by the magnetization characteristics above 10 kOe, that is, the magnetization continuously increases with increasing magnetic field without approaching saturation. The Ferrimagnetic order of a related Mn-based antiperovskite compound was explained by a spin structure, where two of the three Mn magnetic moments are antiferromagnetically coupled and the third exhibits FM behavior [19]. It is possible that a similar magnetic structure is established in Mn_{3}SbN below 353 K.

To further characterize the magnetic transition, the specific heat was measured from 400 to 2 K. As shown in Figure 3, the temperature dependence of features a sharp and narrow peak around (/*R* = 87 and Δ*T* = 3 K, where is the ideal gas constant). This is indicative of a first-order-like transition, as discussed in [20].

An estimation of entropy change is essential to understanding the nature of the transition of Mn_{3}SbN. The peak was roughly separated from the baseline using a polynomial function. Analysis indicates that the total transition entropy () is ~1.23*R* (10.2 J/mol K). Since the total entropy change comprises all contributions, including the lattice, electronic, and magnetic changes [20], we evaluated each contribution independently.

For the present compound, the abrupt change of the magnetization at may induce a large *∂**M*/*∂**T*; therefore, a large magnetic entropy change () is expected. A series of magnetization curves with small temperature steps were measured; the data allow for a rough estimation of the magnetic entropy change via the thermodynamic Maxwell relation, as follows [21]:
The magnetic entropy change, (), can be calculated by
The temperature dependence of calculated from (2) with fields of 10, 20, 30, 40, and 50 kOe is shown in Figure 4. The is maximized around , and the maximum is estimated to be ~2.1 J mol^{−1} K^{−1}, which implies that the lattice and electronic changes provide a fairly large contribution to the total entropy change.

To investigate the electronic contribution (i.e., the Sommerfeld coefficient or ), the versus plot below 10 K was analyzed by applying the approximate Debye model, as follows: = + 2.4*n *(1/) (,), where denotes the number of atoms per formula unit, is the Boltzmann constant, is the Avogadro constant, and is the Debye temperature. Fitting to the linear part of the versus plot using the least-squares method yielded and values of ~7.03 mJ mol^{−1} K^{−2} and 326 K, respectively. Compared with the parameters determined for other antiperovskite nitrides, Mn_{3}SbN has a much lower , which indicates that the electronic correlation is somewhat weakened [20]. Thus, the electronic contribution might not be a dominant contributor to the total transition entropy.

In addition to the magnetic and electronic contributions, a possible lattice change may need to be investigated to analyze the total transition entropy. The variation of the synchrotron XRD pattern with temperature was measured. As shown in Figure 5(b). It can be seen that some typical reflections disappear with temperature, for example, the two reflections (002) and (200) for the *P4*/*mmm * lattice merge to one reflection. By the Rietveld analysis of the synchrotron XRD patterns, the structural change from tetragonal to cubic was defined, and the lattice constants were determined as a function of temperature, as shown in Figure 5(a). It is obvious that lattice parameter increases slightly with increasing temperature, whereas gradually decreases. When the temperature crosses , the tetragonal structure completely transforms to an unidentified cubic structure. Hence, the lattice distortion must contribute to the total entropy change.

According to the thermodynamic relation, the magnetization () is equal to the first derivative of the magnetic free energy by the magnetic field, that is, *df*()/*dH* [22]. Therefore, the sharp transition indicates that the energy barrier in the free energy that separates the paramagnetic and ferromagnetic states is large. Accordingly, and the energy barrier height probably correlate with the electronic density of states, which exhibits a sharp peak near the Fermi level [23]; therefore, the large entropy change is possibly related to the reconstruction of the electronic structure, which could induce the magnetic and structural transition. Since such an electronic reconstruction is often sharply reflected in a curve, the electronic transport properties of Mn_{3}SbN were carefully measured (shown in Figure 6). It is evident that an abnormal drop appears at in the curve, which is indicative of an electronic structure reconstruction. In addition, as shown in the inset of Figure 6, a small hysteresis was observed between the warming and cooling curves; this is in agreement with a first-order transition.

#### 4. Conclusions

In conclusion, the thermodynamic, electromagnetic, and transport properties of antiperovskite Mn_{3}SbN were studied. The phase crystallizes in a tetragonal structure with *a* = *b* = 4.17994(4) Å and *c* = 4.27718(5) Å at room temperature. The measurements revealed a sharp endothermic peak in the curve at 353 K, which corresponds to a large entropy change (~10.2 J mol^{−1} K^{−1}). The present study clearly indicates that the entropy change is accompanied with a Ferrimagnetic transition and lattice distortion as well as a possible electronic structure reconstruction.

#### Conflict of Interests

The authors declare that they have no conflict of interests.

#### Acknowledgments

The authors would like to thank the staff members at BL15XU, the National Institute for Materials Science (NIMS), and SPring-8 for their help in the use of the beamline. The SXRD measurements were performed with the approval of the NIMS Beamline Station (Proposal no. 2011A4502). This study was supported in part by the World Premier International Research Center Initiative of the Ministry of Education, Culture, Sports, Science, and Technology (MEXT); a Grant-in-Aid for Scientific Research grant (no. 22246083) from the Japan Society for the Promotion of Science (JSPS); the Funding Program for World-Leading Innovative R&D on Science and Technology (FIRST Program) of the JSPS; the Advanced Low Carbon Technology Research and Development Program (ALCA) of the Japan Science and Technology Agency (JST).

#### References

- G. W. Wiener and J. A. Berger, “Structure and magnetic properties of some transition metal nitrides,”
*Transactions of the American Institute of Mining, Metallurgical, and Petroleum Engineers*, vol. 203, pp. 360–368, 1955. View at Google Scholar - Y. Sun, Y. C. Wen, L. H. Chu, M. Nie, and C. Wang, “Abnormal thermal expansion in anti-perovskite manganese nitride,”
*Journal of the Chinese Ceramic Society*, vol. 37, no. 5, pp. 73–77, 2009. View at Google Scholar - B. S. Wang, P. Tong, Y. P. Sun et al., “Large magnetic entropy change near room temperature in antiperovskite SnCMn
_{3},”*Environment People Law*, vol. 85, no. 4, Article ID 47004, 2009. View at Publisher · View at Google Scholar · View at Scopus - R. Huang, L. Li, F. Cai, X. Xu, and L. Qian, “Low-temperature negative thermal expansion of the antiperovskite manganese nitride Mn
_{3}CuN codoped with Ge and Si,”*Applied Physics Letters*, vol. 93, no. 8, Article ID 081902, 3 pages, 2008. View at Publisher · View at Google Scholar · View at Scopus - K. Kamishima, T. Goto, H. Nakagawa et al., “Giant magnetoresistance in the intermetallic compound Mn
_{3}GaC,”*Physical Review B*, vol. 63, no. 2, Article ID 024426, 3 pages, 2001. View at Google Scholar · View at Scopus - S. Iikubo, K. Kodama, K. Takenaka, H. Takagi, M. Takigawa, and S. Shamoto, “Local lattice distortion in the giant negative thermal expansion material Mn
_{3}Cu_{1−x}Ge_{x}N,”*Physical Review Letters*, vol. 101, no. 20, Article ID 205901, 4 pages, 2008. View at Publisher · View at Google Scholar · View at Scopus - Y. Sun, C. Wang, Y. C. Wen, K. G. Zhu, and J. T. Zhao, “Lattice contraction and magnetic and electronic transport properties of Mn
_{3}Zn_{1−x}Ge_{x}N,”*Applied Physics Letters*, vol. 91, Article ID 231913, 3 pages, 2007. View at Google Scholar - K. Asano, K. Koyama, and K. Takenaka, “Magnetostriction in Mn
_{3}CuN,”*Applied Physics Letters*, vol. 92, no. 16, Article ID 161909, 3 pages, 2008. View at Publisher · View at Google Scholar · View at Scopus - T. Shimizu, T. Shibayama, K. Asano, and K. Takenaka, “Giant magnetostriction in tetragonally distorted antiperovskite manganese nitrides,”
*Journal of Applied Physics*, vol. 111, Article ID 07A903, 3 pages, 2012. View at Google Scholar - E. O. Chi, W. S. Kim, and N. H. Hur, “Nearly zero temperature coefficient of resistivity in antiperovskite compound CuNMn
_{3},”*Solid State Communications*, vol. 120, no. 7-8, pp. 307–310, 2001. View at Publisher · View at Google Scholar · View at Scopus - Y. Sun, C. Wang, L. Chu, Y. Wen, M. Nie, and F. Liu, “Low temperature coefficient of resistivity induced by magnetic transition and lattice contraction in Mn
_{3}NiN compound,”*Scripta Materialia*, vol. 62, no. 9, pp. 686–689, 2010. View at Publisher · View at Google Scholar · View at Scopus - K. Takenaka and H. Takagi, “Giant negative thermal expansion in Ge-doped anti-perovskite manganese nitrides,”
*Applied Physics Letters*, vol. 87, no. 26, Article ID 261902, 3 pages, 2005. View at Publisher · View at Google Scholar · View at Scopus - Y. Sun, C. Wang, Q. Z. Huang et al., “Neutron diffraction study of unusual phase separation in the antiperovskite nitride Mn
_{3}ZnN,”*Inorganic Chemistry*, vol. 51, no. 13, pp. 7232–7236, 2012. View at Google Scholar - Y. S. Sun, Y. F. Guo, X. X. Wang et al., “Resistive switching phenomenon driven by antiferromagnetic phase separation in an antiperovskite nitride Mn
_{3}ZnN,”*Applied Physics Letters*, vol. 100, Article ID 161907, 4 pages, 2012. View at Google Scholar - C. Wang, L. H. Chu, Q. R. Yao et al., “Tuning the range, magnitude, and sign of the thermal expansion in intermetallic Mn
_{3}(Zn, M)_{x}N (M = Ag, Ge),”*Physical Review B*, vol. 85, Article ID 220103, 5 pages, 2012. View at Google Scholar - B. Song, J. Jian, H. Bao et al., “Observation of spin-glass behavior in antiperovskite Mn
_{3}GaN,”*Applied Physics Letters*, vol. 92, no. 19, Article ID 192511, 3 pages, 2008. View at Publisher · View at Google Scholar · View at Scopus - P. Lukashev, R. F. Sabirianov, and K. Belashchenko, “Theory of the piezomagnetic effect in Mn-based antiperovskites,”
*Physical Review B*, vol. 78, no. 18, Article ID 184414, 5 pages, 2008. View at Publisher · View at Google Scholar · View at Scopus - F. Izumi and K. Momma, “Three-dimensional visualization in powder diffraction,”
*Solid State Phenomena*, vol. 130, pp. 15–20, 2007. View at Publisher · View at Google Scholar · View at Scopus - D. Fruchart and E. F. Bertaut, “Magnetic studies of the metallic perovskite-type compounds of manganese,”
*Journal of the Physical Society of Japan*, vol. 44, no. 3, pp. 781–791, 1978. View at Google Scholar · View at Scopus - J. García, J. Bartolomé, D. González, R. Navarro, and D. Fruchart, “Thermophysical properties of the intermetallic Mn
_{3}MN perovskites II. Heat capacity of manganese zinc nitride: Mn_{3}ZnN and manganese gallium nitride: Mn_{3}GaN,”*The Journal of Chemical Thermodynamics*, vol. 15, no. 11, pp. 1041–1057, 1983. View at Google Scholar · View at Scopus - M. H. Phan and S. C. Yu, “Review of the magnetocaloric effect in manganite materials,”
*Journal of Magnetism and Magnetic Materials*, vol. 308, no. 2, pp. 325–340, 2007. View at Publisher · View at Google Scholar · View at Scopus - A. Fujita, S. Fujieda, Y. Hasegawa, and K. Fukamichi, “Itinerant-electron metamagnetic transition and large magnetocaloric effects in La(Fe
_{x}Si_{1−x})_{13}compounds and their hydrides,”*Physical Review B*, vol. 67, no. 10, Article ID 104416, 2003. View at Google Scholar · View at Scopus - J. P. Jardin and J. Labbe, “Phase transitions and band structure in metallic perovskites (carbides and nitrides),”
*Journal of Solid State Chemistry*, vol. 46, pp. 275–293, 1983. View at Google Scholar